LMucko/crystallography-open-database huggingface dataset:
Structure cristalline d'un nouveau type de cyclohexaphosphate, Cu2 Cs2 P6 O18 .8(H2O)
Averbuch-Pouchot, M - T; Durif, A; Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences, Ser. II (1994-) 318 (1994) 335–340; doi:

data_1007227
_publ_section_title
;
Structure cristalline d'un nouveau type de cyclohexaphosphate, Cu2 Cs2
P6 O18 .8(H2O)
;
_journal_coden_ASTM              CMCAEK
_journal_name_full
;
Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences,
Ser. II (1994-)
;
_journal_page_first              335
_journal_page_last               340
_journal_volume                  318
_journal_year                    1994
_chemical_formula_structural     'Cu2 Cs2 (P6 O18) (H2 O)8'
_chemical_formula_sum            'Cs2 Cu2 H16 O26 P6'
_chemical_name_systematic
;
Dicopper dicaesium cyclo-hexaphosphate octahydrate
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                105.99(5)
_cell_angle_beta                 91.34(5)
_cell_angle_gamma                102.26(5)
_cell_formula_units_Z            1
_cell_length_a                   9.832(3)
_cell_length_b                   8.651(3)
_cell_length_c                   7.615(3)
_cell_volume                     606.1
_refine_ls_R_factor_all          0.029
_cod_original_formula_sum        'H16 Cs2 Cu2 O26 P6'
_cod_database_code               1007227
The Pb (P O3)2-Rb (P O3) phase-equilibrium crystal structure of Pb Rb (P O3)3
Prisset, J - L; Averbuch-Pouchot, M - T; Durif, A; European Journal of Solid State Inorganic Chemistry 31 (1994) 37–46; doi:

data_1007228
_publ_section_title
;
The Pb (P O3)2-Rb (P O3) phase-equilibrium crystal structure of Pb Rb
(P O3)3
;
_journal_coden_ASTM              EJSCE5
_journal_name_full
;
European Journal of Solid State Inorganic Chemistry
;
_journal_page_first              37
_journal_page_last               46
_journal_volume                  31
_journal_year                    1994
_chemical_formula_structural     'Pb Rb (P O3)3'
_chemical_formula_sum            'O9 P3 Pb Rb'
_chemical_name_systematic        'Lead rubidium catena-tris(phosphate(V))'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 103.85(5)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   14.05(3)
_cell_length_b                   17.09(4)
_cell_length_c                   7.228(3)
_cell_volume                     1685.1
_refine_ls_R_factor_all          0.043
_cod_database_code               1007228
Preparation chimique et structure cristalline d'un polyvanadate d'argent hydrate: Ag V O3 . H2 O
Averbuch-Pouchot, M - T; Durif, A; Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences, Ser. II (1994-) 319 (1994) 1319–1324; doi:

data_1007229
_publ_section_title
;
Preparation chimique et structure cristalline d'un polyvanadate
d'argent hydrate: Ag V O3 . H2 O
;
_journal_coden_ASTM              CMCAEK
_journal_name_full
;
Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences,
Ser. II (1994-)
;
_journal_page_first              1319
_journal_page_last               1324
_journal_volume                  319
_journal_year                    1994
_chemical_formula_structural     'Ag (V O3) (H2 O)'
_chemical_formula_sum            'Ag H2 O4 V'
_chemical_name_systematic        'Silver catena-vanadate(V) hydrate'
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.147(2)
_cell_length_b                   3.655(1)
_cell_length_c                   15.763(8)
_cell_volume                     411.8
_refine_ls_R_factor_all          0.037
_cod_original_formula_sum        'H2 Ag O4 V'
_cod_database_code               1007229
Structure cristalline de l'ultraphosphate d'holmium Ho P5 O14
Tranqui, D; Bagieu-Beucher, M; Durif, A; Bulletin de la Societe Francaise de Mineralogie et de Cristallographie (72,1949-100,1977) 95 (1972) 437–440; doi:

data_1007230
_publ_section_title
;
Structure cristalline de l'ultraphosphate d'holmium Ho P5 O14
;
_journal_coden_ASTM              BUFCAE
_journal_name_full
;
Bulletin de la Societe Francaise de Mineralogie et de Cristallographie
(72,1949-100,1977)
;
_journal_page_first              437
_journal_page_last               440
_journal_volume                  95
_journal_year                    1972
_chemical_formula_structural     'Ho (P5 O14)'
_chemical_formula_sum            'Ho O14 P5'
_chemical_name_systematic        'Holmium pentaphosphate *'
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.726(4)
_cell_length_b                   12.710(6)
_cell_length_c                   8.926(4)
_cell_volume                     990.0
_exptl_crystal_density_meas      3.4
_refine_ls_R_factor_all          0.09
_cod_database_code               1007230
Synthesis and crystal structure of cesium-lithium cyclohexaphosphate dihydrate
El Mokhtar, O S M; Rzaigui, M; Said, H; Averbuch-Pouchot, M T; Durif, A; Materials Research Bulletin 30 (1995) 1049–1054; doi:10.1016/0025-5408(95)00072-0

data_1007231
_publ_section_title
;
Synthesis and crystal structure of cesium-lithium cyclohexaphosphate
dihydrate
;
_journal_coden_ASTM              MRBUAC
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              1049
_journal_page_last               1054
_journal_paper_doi               10.1016/0025-5408(95)00072-0
_journal_volume                  30
_journal_year                    1995
_chemical_formula_structural     'Cs3.064 Li3 (P6 O18) (H2 O)1.98'
_chemical_formula_sum            'Cs3.064 H3.96 Li3 O19.98 P6'
_chemical_name_systematic
;
Caesium lithium cyclo-hexaphosphate hydrate (3.1/3/1/1.98)
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                113.39(4)
_cell_angle_beta                 93.83(4)
_cell_angle_gamma                83.00(4)
_cell_formula_units_Z            1
_cell_length_a                   7.938(2)
_cell_length_b                   7.674(2)
_cell_length_c                   9.556(2)
_cell_volume                     530.2
_refine_ls_R_factor_all          0.022
_cod_original_formula_sum        'H3.96 Cs3.064 Li3 O19.98 P6'
_cod_database_code               1007231
Structure du tetrahydrazinium cyclotetraphosphate: (N H2 - N H3)4 P4 O12
Thabet, H; Bdiri, M; Jouini, A; Durif, A; Journal of Solid State Chemistry 101 (1992) 211–220; doi:10.1016/0022-4596(92)90177-W

data_1007232
_publ_section_title
;
Structure du tetrahydrazinium cyclotetraphosphate: (N H2 - N H3)4 P4 O12
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              211
_journal_page_last               220
_journal_paper_doi               10.1016/0022-4596(92)90177-W
_journal_volume                  101
_journal_year                    1992
_chemical_formula_structural     '(N H2 N H3)4 (P4 O12)'
_chemical_formula_sum            'H20 N8 O12 P4'
_chemical_name_systematic        'Tetrahydrazinium cyclotetraphosphate'
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                114.27(1)
_cell_angle_beta                 111.71(1)
_cell_angle_gamma                83.83(1)
_cell_formula_units_Z            1
_cell_length_a                   7.661(1)
_cell_length_b                   7.341(1)
_cell_length_c                   8.518(1)
_cell_volume                     405.2
_exptl_crystal_density_meas      1.8
_refine_ls_R_factor_all          0.025
_cod_database_code               1007232
The calcium-potassium cyclodecaphosphate hexadecahydrate: Ca4 K2 P10 O30 . 16(H2 O)
Averbuch-Pouchot, M-T; Durif, A; Schuelke, U; European Journal of Solid State Inorganic Chemistry 33 (1996) 1091–1100; doi:

data_1007233
_publ_section_title
;
The calcium-potassium cyclodecaphosphate hexadecahydrate: Ca4 K2 P10
O30 . 16(H2 O)
;
_journal_coden_ASTM              EJSCE5
_journal_name_full
;
European Journal of Solid State Inorganic Chemistry
;
_journal_page_first              1091
_journal_page_last               1100
_journal_volume                  33
_journal_year                    1996
_chemical_formula_structural     'Ca4 K2 (P10 O30) (H2 O)16'
_chemical_formula_sum            'Ca4 H32 K2 O46 P10'
_chemical_name_systematic
;
Tetracalcium dipotassium cyclo-decaphosphate 16-hydrate
;
_space_group_IT_number           33
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      33
_symmetry_space_group_name_Hall  'P 2c -2n'
_symmetry_space_group_name_H-M   'P n a 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.773(2)
_cell_length_b                   15.758(3)
_cell_length_c                   19.91409(20)
_cell_volume                     4635.9
_refine_ls_R_factor_all          0.046
_cod_original_formula_sum        'H32 Ca4 K2 O46 P10'
_cod_database_code               1007233
Structure cristalline de la fresnoite
Masse, R; Grenier, J C; Durif, A; Bulletin de la Societe Francaise de Mineralogie et de Cristallographie (72,1949-100,1977) 90 (1967) 20–23; doi:

data_1007234
_publ_section_title              'Structure cristalline de la fresnoite'
_journal_coden_ASTM              BUFCAE
_journal_name_full
;
Bulletin de la Societe Francaise de Mineralogie et de Cristallographie
(72,1949-100,1977)
;
_journal_page_first              20
_journal_page_last               23
_journal_volume                  90
_journal_year                    1967
_chemical_compound_source        'synthetic at 1350 C'
_chemical_formula_structural     'Ba2 Ti Si2 O8'
_chemical_formula_sum            'Ba2 O8 Si2 Ti'
_chemical_name_mineral           Fresnoite
_chemical_name_systematic        'Barium titanium silicate'
_space_group_IT_number           100
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      100
_symmetry_space_group_name_Hall  'P 4 -2ab'
_symmetry_space_group_name_H-M   'P 4 b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.52
_cell_length_b                   8.52
_cell_length_c                   5.21
_cell_volume                     378.2
_refine_ls_R_factor_all          0.12
_cod_database_code               1007234
Determination de la position des atomes d'hydrogene dans l'hydrogrinat Al2 O3, (Ca O)3 (H2 O)6 par resonance magnetique nucleaire et diffraction neutronique
Cohen-Addad, C; Ducros, P; Durif, A; Bertaut, E F; Delapalme, A; Journal de Physique (Paris) 25 (1964) 478–483; doi:10.1051/jphys:01964002505047800

data_1007235
_publ_section_title
;
Determination de la position des atomes d'hydrogene dans l'hydrogrinat
Al2 O3, (Ca O)3 (H2 O)6 par resonance magnetique nucleaire et
diffraction neutronique
;
_journal_coden_ASTM              JOPQAG
_journal_name_full               'Journal de Physique (Paris)'
_journal_page_first              478
_journal_page_last               483
_journal_paper_doi               10.1051/jphys:01964002505047800
_journal_volume                  25
_journal_year                    1964
_chemical_compound_source        synthetic
_chemical_formula_structural     'Al2 O3 (Ca O)3 (H2 O)6'
_chemical_formula_sum            'Al2 Ca3 H12 O12'
_chemical_name_mineral           Hydrogarnet
_chemical_name_systematic        'Dialuminium tricalcium oxide hexahydrate'
_space_group_IT_number           230
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      230
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.57
_cell_length_b                   12.57
_cell_length_c                   12.57
_cell_volume                     1986.1
_refine_ls_R_factor_all          0.13
_cod_original_formula_sum        'H12 Al2 Ca3 O12'
_cod_database_code               1007235
Crystal structures of the three forms of Cs Zn P O4
Blum, D; Durif, A; Averbuch-Pouchot, M T; Ferroelectrics 69 (1986) 283–292; doi:10.1080/00150198608008201

data_1007236
_publ_section_title
;
Crystal structures of the three forms of Cs Zn P O4
;
_journal_coden_ASTM              FEROA8
_journal_name_full               Ferroelectrics
_journal_page_first              283
_journal_page_last               292
_journal_paper_doi               10.1080/00150198608008201
_journal_volume                  69
_journal_year                    1986
_chemical_formula_structural     'Cs Zn (P O4)'
_chemical_formula_sum            'Cs O4 P Zn'
_chemical_name_systematic        'Caesium zinc phosphate(V) - III'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.14(8)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   18.32999(9000)
_cell_length_b                   5.45(4)
_cell_length_c                   9.25(6)
_cell_volume                     924.1
_refine_ls_R_factor_all          0.043
_cod_database_code               1007236
Crystal structures of the three forms of Cs Zn P O4
Blum, D; Durif, A; Averbuch-Pouchot, M T; Ferroelectrics 69 (1986) 283–292; doi:10.1080/00150198608008201

data_1007237
_publ_section_title
;
Crystal structures of the three forms of Cs Zn P O4
;
_journal_coden_ASTM              FEROA8
_journal_name_full               Ferroelectrics
_journal_page_first              283
_journal_page_last               292
_journal_paper_doi               10.1080/00150198608008201
_journal_volume                  69
_journal_year                    1986
_chemical_formula_structural     'Cs Zn (P O4)'
_chemical_formula_sum            'Cs O4 P Zn'
_chemical_name_systematic        'Caesium zinc phosphate(V) - II'
_space_group_IT_number           33
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      33
_symmetry_space_group_name_Hall  'P -2ac -2n'
_symmetry_space_group_name_H-M   'P n 21 a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.236(6)
_cell_length_b                   5.462(3)
_cell_length_c                   9.342(7)
_cell_volume                     471.3
_refine_ls_R_factor_all          0.041
_cod_database_code               1007237
Crystal structures of the three forms of Cs Zn P O4
Blum, D; Durif, A; Averbuch-Pouchot, M T; Ferroelectrics 69 (1986) 283–292; doi:10.1080/00150198608008201

data_1007238
_publ_section_title
;
Crystal structures of the three forms of Cs Zn P O4
;
_journal_coden_ASTM              FEROA8
_journal_name_full               Ferroelectrics
_journal_page_first              283
_journal_page_last               292
_journal_paper_doi               10.1080/00150198608008201
_journal_volume                  69
_journal_year                    1986
_chemical_formula_structural     'Cs Zn (P O4)'
_chemical_formula_sum            'Cs O4 P Zn'
_chemical_name_systematic        'Caesium zinc phosphate(V) - I'
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.194(3)
_cell_length_b                   5.490(2)
_cell_length_c                   9.388(4)
_cell_volume                     473.9
_refine_ls_R_factor_all          0.042
_cod_database_code               1007238
Structure cristalline de l'ultraphosphate de Samarium Sm P5 O14
Tranqui, D; Bagieu, M; Durif, A; Acta Crystallographica B (24,1968-38,1982) 30 (1974) 1751–1755; doi:10.1107/S0567740874005747

data_1007239
_publ_section_title
;
Structure cristalline de l'ultraphosphate de Samarium Sm P5 O14
;
_journal_coden_ASTM              ACBCAR
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              1751
_journal_page_last               1755
_journal_paper_doi               10.1107/S0567740874005747
_journal_volume                  30
_journal_year                    1974
_chemical_formula_structural     'Sm P5 O14'
_chemical_formula_sum            'O14 P5 Sm'
_chemical_name_systematic        'Samarium pentaphosphate'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2bc'
_symmetry_space_group_name_H-M   'P 1 1 21/b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90.45(1)
_cell_formula_units_Z            4
_cell_length_a                   8.750(4)
_cell_length_b                   12.990(6)
_cell_length_c                   8.944(4)
_cell_volume                     1016.6
_refine_ls_R_factor_all          0.05
_cod_database_code               1007239
Les ultraphosphates
Durif, A; Bulletin de la Societe Francaise de Mineralogie et de Cristallographie (72,1949-100,1977) 94 (1971) 314–318; doi:

data_1007240
_publ_section_title              'Les ultraphosphates'
_journal_coden_ASTM              BUFCAE
_journal_name_full
;
Bulletin de la Societe Francaise de Mineralogie et de Cristallographie
(72,1949-100,1977)
;
_journal_page_first              314
_journal_page_last               318
_journal_volume                  94
_journal_year                    1971
_chemical_formula_structural     'Ho P5 O14'
_chemical_formula_sum            'Ho O14 P5'
_chemical_name_systematic        'Holmium phyllo-pentaphosphate'
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.72
_cell_length_b                   12.71
_cell_length_c                   8.926
_cell_volume                     989.3
_cod_database_code               1007240
Etude systematique des phosphates condenses
Laugt, M; Durif, A; Seminaire de Chimie de l'Etat Solide 1971-72 1972 (1972) 157–175; doi:

data_1007241
_publ_section_title              'Etude systematique des phosphates condenses'
_journal_coden_ASTM              SESOLV
_journal_name_full
;
Seminaire de Chimie de l'Etat Solide 1971-72
;
_journal_page_first              157
_journal_page_last               175
_journal_volume                  1972
_journal_year                    1972
_chemical_formula_structural     'Li Cu (P O3)3'
_chemical_formula_sum            'Cu Li O9 P3'
_chemical_name_systematic        'Lithium copper catena-phosphate'
_space_group_IT_number           19
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      19
_symmetry_space_group_name_Hall  'P 2ac 2ab'
_symmetry_space_group_name_H-M   'P 21 21 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.703
_cell_length_b                   8.197
_cell_length_c                   8.613
_cell_volume                     614.4
_cod_database_code               1007241
Etude systematique des phosphates condenses
Laugt, M; Durif, A; Seminaire de Chimie de l'Etat Solide 1971-72 1972 (1972) 157–175; doi:

data_1007242
_publ_section_title              'Etude systematique des phosphates condenses'
_journal_coden_ASTM              SESOLV
_journal_name_full
;
Seminaire de Chimie de l'Etat Solide 1971-72
;
_journal_page_first              157
_journal_page_last               175
_journal_volume                  1972
_journal_year                    1972
_chemical_formula_structural     'K2 Cu (P O3)4'
_chemical_formula_sum            'Cu K2 O12 P4'
_chemical_name_systematic        'Dipotassium copper catena-phosphate'
_space_group_IT_number           9
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      9
_symmetry_space_group_name_Hall  'C -2yc'
_symmetry_space_group_name_H-M   'C 1 c 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.49
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.94
_cell_length_b                   12.25
_cell_length_c                   7.904
_cell_volume                     1041.6
_cod_database_code               1007242
Structure du trimetaphosphate-tellurate de sodium hexahydrate Te (O H)6 (Na3 P3 O9)2 (H2 O)6
Boudjada, N; Averbuch-Pouchot, M T; Durif, A; Acta Crystallographica B (24,1968-38,1982) 37 (1981) 645–647; doi:10.1107/S0567740881003762

data_1007243
_publ_section_title
;
Structure du trimetaphosphate-tellurate de sodium hexahydrate Te (O H)6
(Na3 P3 O9)2 (H2 O)6
;
_journal_coden_ASTM              ACBCAR
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              645
_journal_page_last               647
_journal_paper_doi               10.1107/S0567740881003762
_journal_volume                  37
_journal_year                    1981
_chemical_formula_structural     '(Te (O H)6) (Na3 P3 O9)2 (H2 O)6'
_chemical_formula_sum            'H18 Na6 O30 P6 Te'
_chemical_name_systematic
;
Tellurium hexahydroxide - trisodiumcyclo-triphosphate - water (1/2/6)
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      176
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   11.67(1)
_cell_length_b                   11.67(1)
_cell_length_c                   12.12(1)
_cell_volume                     1429.5
_refine_ls_R_factor_all          0.04
_cod_database_code               1007243